text: The movement of grain boundaries (HAGB) has implications for recrystallization and grain growth while subgrain boundary (LAGB) movement strongly influences recovery and the nucleation of recrystallization.
  A boundary moves due to a pressure acting on it. It is generally assumed that the velocity is directly proportional to the pressure with the constant of proportionality being the mobility of the boundary. The mobility is strongly temperature dependent and often follows an Arrhenius type relationship:
  The apparent activation energy (Q) may be related to the thermally activated atomistic processes that occur during boundary movement. However, there are several proposed mechanisms where the mobility will depend on the driving pressure and the assumed proportionality may break down.
  It is generally accepted that the mobility of low-angle boundaries is much lower than that of high-angle boundaries. The following observations appear to hold true over a range of conditions:
  * The mobility of low-angle boundaries is proportional to the pressure acting on it.
  * The rate controlling process is that of bulk diffusion
  * The boundary mobility increases with misorientation.
  Since low-angle boundaries are composed of arrays of dislocations and their movement may be related to dislocation theory. The most likely mechanism, given the experimental data, is that of dislocation climb, rate limited by the diffusion of solute in the bulk.
  The movement of high-angle boundaries occurs by the transfer of atoms between the neighbouring grains. The ease with which this can occur will depend on the structure of the boundary, itself dependent on the crystallography of the grains involved, impurity atoms and the temperature. It is possible that some form of diffusionless mechanism (akin to diffusionless phase transformations such as martensite) may operate in certain conditions. Some defects in the boundary, such as steps and ledges, may also offer alternative mechanisms for atomic transfer.
  Since a high-angle boundary is imperfectly packed compared to the normal lattice it has some amount of free space or free volume where solute atoms may possess a lower energy. As a result, a boundary may be associated with a solute atmosphere that will retard its movement. Only at higher velocities will the boundary be able to break free of its atmosphere and resume normal motion.
  Both low- and high-angle boundaries are retarded by the presence of particles via the so-called Zener pinning effect. This effect is often exploited in commercial alloys to minimise or prevent recrystallization or grain growth during heat-treatment.